COMPUTER SIMULATION OF DRAWING PROCESS WITH SHEAR
Chief researcher, Candidate of Science (Engineering) Semenov V.I., junior researcher Raab A.G.
Institute of Physics of Advanced Materials – Ufa State Aviation Technical University, Ufa, Russia
Abstract: With the help of computer simulation in the software “DEFORM-3D” there was performed virtual complete factor experiment of
the drawing with shear process, in its course there was performed assessment of influence of independent parameters (drawing speed, die
rotation speed, die angle and friction factor) on the strain intensity. As a result of the experiment there was derived a regression equation
and were determined the most significant individual factors and their combination, which influence the response parameters. Also, there
were represented the comparative results of processes of conventional drawing and shear drawing. There was demonstrated a higher
efficiency of shear drawing process from the point of view of strain intensity.
KEYWORDS: COMPUTER SIMULATION, SHEAR DRAWING, VIRTUAL COMPLETE FACTOR EXPERIMENT, PLANNING MATRIX,
At present time there is observed a considerable interest to studies
in the sphere of strength increase of metals by means of structure
refinement to submicrocrystalline (SMC) dimensions via
processing under conditions of severe plastic deformation (SPD)
. One of the most advanced techniques of SPD is multicycle
equal channel angular pressing (ECAP) [2, 3] and its further
development - ECAP-Conform , designed for production of
long-length billets with a bulk SMC structure and allowing creating
background for practical realization of the SPD process.
Technological process, based on structure refinement by the SPD
technique and realized on the ECAP-conform die-set is a highly
efficient technique of strength increase of metals and alloys.
However this technique has a number of drawbacks:
1) multicycle processing for achievement of high values of
accumulated strain, which is the basis for strength increase of the
2) production of long-length rods with a square cross section;
3) introduction of additional post-processing treatment, for example
drawing (calibration), for getting rods with a round cross section.
2. Background for solution of the problem
For elimination of the mentioned drawbacks there is suggested the
method of drawing with shear. The invention is designed for
formation of a SMC structure and increase of a complex of
mechanical properties in long-length metallic materials with the
length to diameter ratio of over 100 by means of deformation
processing. The method comprises drawing with shear and
deformation of the metal by means of application of the tractive
force via two successive conical drawing dies with simultaneous
rotation of one of the drawing dies. Performance of the low-cost
production deformation process, accompanied by change of
physical-mechanical properties of metal is achieved by means of
providing of additional shear strain by the set eccentricity in
relation to the axis of rotation, formed by the conical channel of the
rotating drawing die .
The behavior description and forecasting of the process of drawing
with shear is complicated due to the lack of full-scale experiments,
as work on physical experiments is both time and money-
In the scientific and practical activity a significant place is occupied
by numerical methods of complex processes study, including
computer simulation with application of the up-to-date software.
However efficiency of application of simulation techniques and
solution of engineering tasks considerably increases if on the stage,
preceding to the design of the real technological process, there are
created conditions for assessment of value of the most important
Application of mathematical methods for simulation of labor-
intensive and high-cost experiments is one of the most rational
approaches to solution of tasks on assessment of efficiency of non-
standard forming processes. Therefore it appears reasonable to
perform numerical simulation with planning of virtual complete
factor experiment by the “path-of-steepest-ascent” method .
The advantage of the factor experiment is the possibility to describe
the process with complete compliance with the algorithm of the
physical experiment taking into account the set assumptions. The
complete factor experiment is the most easily realizable one among
numerous methods of physical experiment. The aim of application
of the complete factor experiment is getting the linear mathematic
model of the process, which allows determining the further strategy
for performance of the real experiment.
Thus, the aim of the simulation is performance of the virtual process
of drawing with shear with the help of the complete factor
experiment, and determination of the most efficient drawing regime
for production of long-length SMC semi-products.
3. Investigation technique
For obtaining the possibly most complete information about the
investigated dependencies the complete factor experiment was used
in performance of simulation. Planning of the experiment is a
procedure of choice of the number and conditions of experiments,
necessary and sufficient for getting the mathematic model of the
process . However it is important to take into account the
following: tendency to minimize the number of experiments;
simultaneous varying of all variables, determining the process;
choice of a distinct strategy, allowing making justified decisions
after every set of experiments. Prior to performance of planning a
full-scale experiment it is necessary to collect additional
information on the investigated issue; all experience and
knowledge, obtained in the earlier investigations or described in
literature, are used for getting this information .
Planning of the experiment was performed on the method of
production of long-length steel rods with a round cross-section by
drawing with shear, performed on a drawing die-set with a drawing
device consisting of two rotating dies  fig.1.
Fig. 1. Dies for drawing with shear.
The subject of the research is a low-carbon steel with the content of
carbon of 0.1 %, its rheological properties were set for development
of the numerical model .
For realization of the numerical simulation procedure the standard
software application package (SAP) «DEFORM-3D» was used.
With the view of performance of simulation and factor experiment
in the SAP «DEFORM-3D» there were preliminary created bulk
models of dies with various approach angles in the software product
3.1. Taken assumptions
1) billet material in the initial condition (prior to deformation)
is isotropic, there are no initial stresses and strains in it;
2) deformation environment temperature is 20ºС;
3) the tool is absolutely rigid, automated consideration of the
4) initial billet material is plastic;
5) prior to start of simulation, the die, which is a movable tool,
was set with the rotating speed of 1.5 mm/sec along the drawing
axis, and also the rotation frequency of 10 rad. There were chosen
100 steps for simulation, reflecting complete passing of the billet
through the dies and getting of a stable result;
6) The billet was divided into 43553 elements in the form of
On the stage of preparation of the simulation task we consider that
the most significant factors, influencing the strain intensity during
drawing with shear at room temperature are: wire drawing speed V
(Х1), die rotation speed ω (Х2), die approach angle α (Х3), and
friction factor ffr. (Х4). These factors were taken as independent
variables. The response parameter (the dependent variable) was
used for determining the material strain intensity (Y). Therefore it
was decided to perform a virtual complete factor experiment with
application of a two-level model with four unknowns, in accordance
with the number of variable factors, with subsequent formalization
of the obtained results in the form of regression equation and
optimization of the chosen factors.
Every factor was varied on two levels. The variability intervals of
the variable factors and their full-scale values are represented in
Levels of factors
Factors X1 (V, m/min) X2 (ω, min-1
) X3 (α, deg) X4 (ffr.)
Main level (Xi) 20 350 15 0.50
Variability interval (Xi) 10 50 5 0.25
Upper level (xi = 1) 30 600 20 1
Lower level (xi = – 1) 10 100 10 0
The coded values of the numerical factors (xi) are connected with
the full-scale ones (Xi) by the ratios:
It is necessary to define such values of V, ω, α, ffr., which provide
getting the strain intensity ε within the range of values from 1 to 3,
(1 ≤ ε ≤ 3).
The number of experiments N was determined by the number of
factors k in accordance with the expression:
4. Experiment results and discussion
The mathematic model after realization of the experiments of the
complete factor experiment has the view:
y = b0 + b1x1 + b2x2 +…+ b12x1x2 + b13x1x3 +…
+ b123x1x2x3 + b124x1x2x4 + …+ b1234x1x2x3x4, (3)
where bi – regression coefficients.
For calculation of this model coefficients an augmented matrix of
planning and of experiment results was plotted (table 2).
Augmented matrix of plan 24
and experiment results
х0 х1 х2 х3 х4 х1х2 х1х3 х1х4 х2х3 х2х4 х3х4 х1х2х3 х1х2х4 х1х3х4 х2х3х4 х1х2х3х4 у
1 + + + + + + + + + + + + + + + + 0.30
2 + - + + + - - - + + + - - - + - 0.70
3 + + - + + - + + - - + - - + - - 0.90
4 + - - + + + - - - - + + + - - + 0.50
5 + + + - + + - + - + - - + - - - 0.50
6 + - + - + - + - - + - + - + - + 0.90
7 + + - - + - - + + - - + - - + + 0.60
8 + - - - + + + - + - - - + + + - 0.70
9 + + + + - + + - + - - + - - - - 0.40
10 + - + + - - - + + - - - + + - + 1.50
11 + + - + - - + - - + - - + - + + 1.10
12 + - - + - + - + - + - + - + + - 1.20
13 + + + - - + - - - - + - - + + + 0.70
14 + - + - - - + + - - + + + - + - 0.90
15 + + - - - - - - + + + + + + - - 1.30
16 + - - - - + + + + + + - - - - + 1.00
The regression coefficients were calculated by the formula:
ib , (4)
where i = 0, 1, 2, …, 16.
As a result of the performed calculations there was obtained the
general view of the linear equation of regression:
y = 0.825X0 + 0.0125X1 + 0.2X2 – 0.1125X3 – 0.075X4 –
0.1625X1X2 – 0.05X1X3 +0.175X1X4 – 0.0125X2X3 + 0.05X2X4 –
0.0375X3X4 +0.05X1X2X3 – 0.0875X1X2X4 + 0.0X1X3X4 +
0.0625X2X3X4 + 0.0X1X2X3X4 (5)
By analysis of the equation (5) there was determined the statistical
significance of every one of the 16 regression coefficients.
As in this case there was used a uniform duplication of experiments,
the dispersion of coefficient estimates was calculated by the
S , (6)
yS = 0.0137 – experiment dispersion, calculated by the
known techniques . Therefrom
S = 0.00086, and the root-
ibS = 0.0293.
In case of significance level = 0.05 and the number of degrees of
freedom f1 = N = 16 the table value of the t-Student criterion t0.05; 16
= 2.12 . Then the confidence interval of the regression
0621.01i ;b ibf St . (7)
Coefficients, the absolute value of which is equal or higher than the
confidence interval bi
ib , are accepted as statistically
significant . In this case bi 0.0621, i.e. these are b2, b3, b4, b12,
b14, b124, b234.
Statistically insignificant coefficients b1, b13, b23, b24, b34, b123, b134,
b1234 were removed from the equation (5), and after realization of
the complete factor experiment 24
the regression equation got the
y = 0.825X0 + 0.2X2 – 0.1125X3 – 0.075X4 + 0.1025X1X2
+0.175X1X4 – 0.0875X1X2X4 + 0.0625X2X3X4 (8)
Hypothesis of adequacy of the model was checked with the help of
F-ratio test. With the help of the equation (8), there were
determined the calculated values уcalc and then they were compared
with the experimental values уexp (table 3).
Comparison of the experimental and calculated data
Уexp Уcalc /у/ у2
1 0.30 0.425 0.125 0.015625
2 0.70 0.575 0.125 0.015625
3 0.90 0.715 0.175 0.030625
4 0.50 0.355 0.145 0.021025
5 0.50 0.475 0.025 0.000625
6 0.90 0.825 0.075 0.005625
7 0.60 0.575 0.025 0.000625
8 0.70 0.685 0.015 0.000225
9 0.40 0.375 0.025 0.000625
10 1.50 1.550 0.050 0.002500
11 1.10 1.175 0.075 0.005625
12 1.20 1.150 0.050 0.002500
13 0.70 0.675 0.025 0.000625
14 0.90 1.075 0.175 0.030625
15 1.30 1.150 0.150 0.022500
16 1.00 1.150 0.150 0.022500
As duplication of the experiments was uniform, the dispersion of
inadequacy was determined by the formula:
where f2 = N – k’ – number of degrees of freedom, k’ – number of
remained equation coefficients (including b0). The obtained model
(8) comprised 8 coefficients, thus the number of freedom degrees f2
= 8, and dispersion of inadequacy
inadS = 0.0222.
The calculated value of the F-ratio was determined by the formula:
F-ratio value represents the ratio of the dispersion of inadequacy to
dispersion of the experiment and answers the question, by how
many times the model forecasts worse than the experiment.
The hypothesis of adequacy of the equation is accepted in case
when the calculated value of the F-ratio does not exceed the table
value for the selected level of significance, i.e. when Fcalc
The calculated value of the F-ratio
16;8F = 1.62, in case of the
level of significance = 0.05 the table value of the F-ratio
16;8;05.0F = 2.64.
the hypothesis of adequacy of the mathematic
model (8) with the 5 % level of significance is not rejected.
From the equation (8) it is seen that the most significant influence
on the value of strain intensity is made by the die rotation speed, die
approach angle and friction factor, and also joint interaction of the
drawing speed and die rotation speed, drawing speed and friction
factor, drawing speed, die rotation speed and friction factor, die
rotation speed, die approach angle and friction factor. The joint
interaction of other factors has insignificant influence on the value
of strain intensity. With that it is established that with the increase
of the die rotation speed and reduction of the die approach angle
and friction factor the strain intensity increases. Also the response
parameter increases in case of simultaneous increase of drawing
speed and die rotation speed. A more significant influence on strain
intensity is made by joint increase of the drawing speed and the
friction factor. To a lesser degree there is expected influence of
simultaneously three independent variables considered here:
drawing speed, die rotation speed and friction factor, and also die
rotation speed, die approach angle and friction factor. With that
their total action is differently directed. In any case complex
interactions should be analyzed on a case-by-case basis and with
reference to the specific conditions of operation of the multi-
From the equation (8) it is seen that the drawing speed per se has a
slight influence on strain intensity, but in combination with the die
rotation speed, die approach angle and contact conditions in the
plastic triboconjunction can efficiently increase the strain intensity.
Therefore, the maximum value of strain intensity can be obtained in
case of optimum combination of drawing speed with other
independent parameters, considered in this investigation.
For analysis of the obtained mathematic model there was plotted the
diagram of influence of the investigated factors on strain intensity
In fig. 2 it is observed that the biggest influence on strain intensity
is made by the die rotation speed. The strain intensity increases with
the growth of rotation speed. The drawing speed has a very small
influence on the value of strain intensity, however the combination
of the processing speed with the die rotation speed has a significant
influence on the response parameter.
Fig. 2. Influence of significant factors and their interrelations:
negative values – in case of factor decrease the response parameter
increases; positive values – in case of factor increase the response
From this it can be concluded that the efficiency of the process of
drawing with shear depends on synchronization of these two
parameters, which should be considered jointly for design planning
of the technological process. In fig. 2 it is also seen that the die
approach angle and the friction factor, as individual parameters,
should decrease for increase of the strain intensity. From the
analysis of the couple and triple effects of interaction (Х1Х4, Х1Х2Х4,
Х2Х3Х4), it is seen that the friction factor and the die approach angle
in combination with the die rotation speed have significant and
complex influence on strain intensity, which should be taken into
account for design planning of the technological process of drawing
Of practical interest is the solution of the optimization task on
determination of actual values of independent parameters,
considered in the virtual experiment of numerical simulation,
providing maximum value of strain intensity in case of drawing
with shear. This task was solved by the “path-of-steepest ascent”
In accordance with this method the movement from a certain point
inside the investigated area in direction of the gradient i.e. in
direction of the biggest derivative of the response function – is the
shortest way to extreme point. In case of presence of the linear
model for performance of movement by the gradient it is necessary
to vary factor values proportionally to the coefficient values b1, b2,
b3, b4 taking into account their modifying sign.
Steps in variation of factors were calculated in full-scale. Firstly
there were determined the multiplications of coefficients to the
corresponding intervals of variation of the factors, (biXi), then in
proportion to these products there were set steps. The orders of
realization of the stages of the path-of-steepest-ascent are
represented in table 4.
As the characteristics of the stress-strain condition, having a
significant influence on strain intensity, are die rotation speed, die
approach angle and friction factor (the drawing speed influence in
the investigated range was considered as statistically insignificant),
the three factors mentioned above were taken as main factors,
subject to variation.
The values biXi, were used for determining the steps of factor
variation in the following way:
As the response function is the value of strain intensity, the steps in
direction opposite to their modifying signs will decrease the value
of function y.
X2 (die rotation
Step after rounding-off
Main level (Xi) 20 350 15 0.50
value biXi for Х1 (drawing speed) was set a priori due to the necessity to synchronize this factor with other independent variable
parameters, taken for consideration. The step was chosen at random due to technological reasons
Some of the thought experiments were realized in the computer
model (table 4). The experiment planning with application of the
path-of-steepest-ascent method demonstrated that under the
investigated conditions the highest strain intensity will be at high
speed of die rotation (ω ≈ 600 min-1
), low die approach angle (α ≈
) and the decreasing friction factor (ffr. → min). With that the
axial drawing speed (V), due to the low influence on the strain
intensity as an individual parameter was taken as constant and equal
to 15 m/min.
Within the frames of the set investigation task there were obtained
optimized values of the variable parameters, corresponding to the
required value of strain intensity (ε ≥ 1.5): V = 15 m/min; V1 = 500
rot/min; α = 16°.
By insertion of the obtained values into the new model, with other
conditions being equal, we get the distribution fields of stresses and
strains, and also the corrected value of strain intensity. Simulation
of the process of drawing with shear in the «DEFORM 3D» was
performed with the following adjusted parameters:
Friction factor (Siebel) 0.12
Die approach angle, deg 16
Drawing speed, m/min 15
Die rotation speed, min-1
Below there are represented results of numerical simulation by the
optimized values, obtained in the course of performance of virtual
complete factor experiment.
Investigation of the deformed condition of the billet after drawing
with shear demonstrates that the level of strain intensity after
passing of the billet through the die has a nonhomogeneous state.
This strain makes ε = 0.5 – 1.6, which testifies to the severe
character of impact on the material of the initial billet after one pass
through the dies (fig. 3, 4а, 5а,).
The highest value is achieved on the billet surface, as the highest
strain of metal related to the die geometry and their rotation method
in relation to the drawing axis takes place there.
Fig. 3 Image of distribution of strain intensity of the process of
drawing with shear: а – in the longitudinal section on the billet
axis; b – in the longitudinal section on the surface of the billet.
For estimation of values of strain intensity per one processing cycle
there was performed control comparative analysis of the two
processes – drawing with shear and conventional drawing
In the images of distribution of strain intensity (fig. 4) and normal
forces on the deforming tool (fig. 5) it is observed that the process
of drawing with shear is a more preferable one from the point of
view of strain intensity per one drawing cycle.
Fig. 4 Image of strain intensity in the cross section: а – process of
drawing with shear; b – conventional drawing.
Fig. 5 Distribution of normal forces on the deforming tool. а –
drawing with shear; b – conventional drawing.
Investigation of normal forces on the tool demonstrate that during
rotation of the die, the forces on the tool decrease by almost 2
times, which gives the most wide range of choice of steel for
fabrication of the tool and may contribute to cheapening of the
process (fig. 5).
The graphs represented in fig. 6 demonstrate the results of
comparative analysis of the two processes. It is seen that per one
cycle of processing by drawing with shear it is possible to get
significantly higher values of strain intensity and by means of it to
increase the efficiency of the process of fabrication of high-strength
products due to efficient formation of the SMC structure.
Fig. 6 Comparative graphs of values of strain intensity, obtained in
the course of drawing with shear and in the course of conventional
1. Virtual complete factor experiment by the path-of-steepest-
ascent method allowed determining the optimum numerical values
of independent parameters, providing maximum value of strain
intensity at room temperature. Thus, for getting ε ≈ 1.6 it is
necessary to provide the die rotation speed of ω ≈ 500 min-1
approach angle α ≈ 16 о
and friction factor ffr. ≈ 0.12 with the
drawing speed of V = 15 m/min.
2. The comparative analysis of the processes of drawing with
shear and conventional drawing of steel 10 at room temperature
allows decreasing the drawing forces by almost 2 times, increasing
nonhomogeneity of deformation and maximum values of
accumulated strain intensities from 0.5 to 1.6 and moreover, to
decrease normal forces on the tool by 1.8 times.
The work was done within the frames of the project № 11-08-
97038-р_povoljie_а, supported by RFBR and AS RB.
. Valiev R.Z. Bulk nanostructured metallic materials: production,
structure and properties/R.Z. Valiev, I.V. Alexandrov – М.: IKC
«Academkniga», 2007. – 398 p.
. Segal V.M., Reznikov V.I., Kopylov V.I. et al. Processes of
plastic structureformation of metals. Minsk: Science and
engineering, 1994. 232 p.
. Segal V.M. Engineering and commercialization of equal
channel angular extrusion // Mater. Sci. Eng. A. – 2004; V.
386.P. 269 – 276
. Raab G.I., Valiev R.Z. Equal channel angular pressing of long-
length billets. Non-ferrous metallurgy -2000 -№5, с.50-53
. Patent on invention № 2347633 Method of production of
ultrafine grained semi-products by drawing with shear. Published
27.02.2009 Inventors: Raab G.I., Raab A.G. Patent holder: SEI
HPE USATU, valid.
. Novik F.S., Arsov Y.B. Optimization of processes of metal
technology by methods of experiment planing.-М.: Machine-
building; Sofia: Technique. 1980. 304 p.
. Adler Y.P. Pre-planning of experiment. М.: Znanie. 1978. 72 p.
. Adler Y.P. Introduction to experiment planning М.: Metallurgy.
1969. 158 p.
. Classifier of steels and alloys/ V.G. Sorokin, A.V. Volosnikova,
S.A. Vyatkin et al. М.: Machine building. 1989. 640 p.
. Slavutskiy L.A. Basic of data registration and experiment
planning: manual. Cheboksary: ed. ChGU, 2006. 200 p.